# Stability of Cu-Precipitates in Al-Cu Alloys

^{1}

^{2}

^{3}

^{4}

^{*}

^{†}

## Abstract

**:**

## 1. Introduction

## 2. Methods: Computational Schemes

**k**-point mesh [32]. Employing the 108-atom supercell for face-centered cubic (fcc) Al we compare the results obtained with $4\times 4\times 4$ and $6\times 6\times 6$

**k**-point meshes to check the convergence of the total energy. Differences in the total energy of the systems are less than $5\phantom{\rule{0.166667em}{0ex}}\mathrm{meV}$ per atom. All the calculations have thereafter been performed with the finer MP-mesh. A plane-wave cutoff of $300\phantom{\rule{0.166667em}{0ex}}\mathrm{eV}$ is used in the calculation of the pseudo valence wave functions.

## 3. Results

#### 3.1. Reliability of Modeling

**k**-point meshes, we have computed the solubility enthalpy of Cu in Al. It is calculated as

#### 3.2. Impurity-Cluster Binding Energies

**k**-point mesh. All the supercell sizes lead to a binding energy of around $50\phantom{\rule{0.166667em}{0ex}}\mathrm{meV}$. For the 128 atom supercell the binding energy is the smallest one reflecting the small spacing between the adjacent Cu habit planes of the periodic images and the ensuing artificial interaction.

#### 3.2.1. 2D-Cu-Clusters in 108-atom Supercells

#### 3.2.2. 2D-Cu-Clusters in 128- and 192-atom Supercells

#### 3.2.3. Lattice Relaxations

#### 3.2.4. Relaxed Versus Static Configurations

#### 3.2.5. Comparison with Zinc Clusters

#### 3.2.6. Pre-Guinier-Preston Zones in Al-Cu and Al-Zn

## 4. Discussion and Conclusions

## Author Contributions

## Funding

## Acknowledgments

## Conflicts of Interest

## Abbreviations

PAS | Positron Annihilation Spectroscopy |

XAFS | X-ray Absorption Fine Structure |

DFT | Density Functional Theory |

LDA | Local Density Approximation |

GGA | General Gradient Approximation |

VASP | Vienna Ab initio Simulation Package |

PAW | Projector Augmented Wave |

MP | Monkhorst-Pack |

SIESTA | Spanish Initiative for Electronic Simulations with Thousands of Atoms |

DZP | Double Zeta Polarized |

1NN | Nearest Neighbors |

2NN | Next Nearest Neighbors |

XRD | X-Ray Diffraction |

TEM | Transmission Electron Microscopy |

HR-TEM | High resolution Transmission Electron Microscopy |

fcc | face-centered cubic |

hcp | hexagonal closed-packed |

## References

- Polmear, I. Light Alloys—From Traditional Alloys to Nanocrystals, 4th ed.; Elsevier: Amsterdam, The Netherlands, 2006. [Google Scholar]
- Ostermann, F. Anwendungstechnologie Aluminium, 3rd ed.; Springer: Berlin/Heidelberg, Germany, 2014. [Google Scholar]
- Haasen, P. Physical Metallurgy, 3rd ed.; Cambridge University Press: Cambridge, UK, 1996. [Google Scholar]
- Dupasquier, A.; Folegati, P.; de Diego, N.; Somoza, A. Current positron studies of structural modifications in age-hardenable metallic systems. J. Phys. Condens. Matter
**1998**, 10, 10409–10422. [Google Scholar] [CrossRef] - Guinier, A. La diffraction de rayon X aux tres petis angles: Application a l’etude de phenomenes ultramicroscopiques. Ann. Phys.
**1938**, 12, 161–237. [Google Scholar] - Preston, G. The Diffraction of X-Rays by an Age-Hardening Aluminum and Copper Alloys. Proc. R. Soc. Lond. Ser. A Math. Phys. Sci.
**1938**, 167, 526–538. [Google Scholar] [CrossRef] - Preston, G. The Diffraction of X-Rays by an Age-Hardening Alloy of Aluminum and Copper: The Structure of an Intermediate Phase. Lond. Edinb. Dublin Philos. Mag. J. Sci.
**1938**, 26, 855–871. [Google Scholar] [CrossRef] - De Geuser, F.; Bley, F.; Denquin, A.; Deschamps, A. Mapping the microstructure of a friction-stir welded (FSW) Al-Li-Cu alloy. J. Phys.: Conf. Ser.
**2010**, 247, 012034. [Google Scholar] [CrossRef][Green Version] - De Geuser, F.; Bley, F.; Deschamps, A. A new method for evaluating the size of plate-like precipitates by small-angle scattering. J. Appl. Cryst.
**2012**, 45, 1208–1218. [Google Scholar] [CrossRef] - Decreus, B.; Deschamps, A.; Donnadieu, P.; Ehrström, J.C. On the Role of Microstructure in Governing Fracture Behavior of an Aluminum-Copper-Lithium Alloy. Mater. Sci. Eng. A
**2013**, 586, 418–427. [Google Scholar] [CrossRef] - Le Jolu, T.; Morgeneyer, T.; Denquin, A.; Sennour, M.; Laurent, A.; Besson, J.; Ourgues-Lorenzon, A.F. Microstructural Characterization of Internal Welding Defects and their Effect on the Tensile Behaviour of FSW Joints of AA2198 Al-Cu-Li Alloy. Metall. Mater. Trans. A
**2014**, 45A, 5531–5544. [Google Scholar] [CrossRef] - Bourgeois, L.; Dwyer, C.; Weyland, M.; Nie, J.F.; Muddle, B. Structure and Energetics of the Coherent Interface between the Θ
^{′}Precipitate Phase and Aluminium in Al-Cu. Acta Mater.**2011**, 59, 7043–7050. [Google Scholar] [CrossRef] - Zhang, Y.; Zhang, Z.; Medhekar, N.; Bourgeois, L. Vacancy-tuned Precipitation Pathways in Al-1.7 Cu-0.025In-0.025Sb (at.%) Alloy. Acta Mater.
**2017**, 141, 341–351. [Google Scholar] [CrossRef] - Carling, K.; Wahnström, G.; Mattsson, T.; Sandberg, N.; Grimvall, G. Vacancy Concentration in Al from Combined first-principles and Model Potential Calculations. Phys. Rev.
**2003**, B67, 054101. [Google Scholar] [CrossRef] - Carling, K.; Wahnström, G.; Mattsson, T.; Mattsson, A.; Sandberg, N.; Grimvall, G. Vacancies in Metals: From first-principles Calculations to Experimental Data. Phys. Rev. Lett.
**2000**, 85, 3862–3865. [Google Scholar] [CrossRef] [PubMed] - Ullmaier, H. (Ed.) Landolt-Börnstein—Numerical Data and Functional Relationships in Science and Technology—New Series—Group III: Crystal and Solid State Physics Volume 25: Atomic Defects in Metals; Springer: Berlin, Germany, 1991. [Google Scholar]
- Wolverton, C.; Ozoliņŝ, V. First-principles Aluminum Database: Energetics of Binary Al Alloys and Compounds. Phys. Rev.
**2006**, B73, 144104. [Google Scholar] [CrossRef] - Wolverton, C. Solute-Vacancy Binding in Aluminum. Acta Mater.
**2007**, 55, 5867–5872. [Google Scholar] [CrossRef] - Shin, D.; Wolverton, C. First-principles Study of Solute-Vacancy Binding in Magnesium. Acta Mater.
**2010**, 58, 531–540. [Google Scholar] [CrossRef] - Haaks, M.; Staab, T. High Momentum Analysis in Doppler Spectroscopy. Appl. Surf. Sci.
**2008**, 255, 84–88. [Google Scholar] [CrossRef] - Klobes, B.; Staab, T.; Haaks, M.; Maier, K.; Wieler, I. The Role of Quenched-in Vacancies for the Decomposition of Aluminium Alloys. Phys. Status Solidi (RRL) Rapid Res. Lett.
**2008**, 2, 224–226. [Google Scholar] [CrossRef] - Klobes, B.; Korff, B.; Balarisi, O.; Eich, P.; Haaks, M.; Maier, K.; Sottong, R.; Hühne, S.M.; Mader, W.; Staab, T. Probing the Defect State of Individual Precipitates Grown in an Al-Mg-Si Alloy. Phys. Rev.
**2010**, B82, 054113. [Google Scholar] [CrossRef] - Klobes, B.; Maier, K.; Staab, T. Natural Ageing of Al-Cu-Mg Revisited from a Local Perspective. Mater. Sci. Eng. A
**2011**, 528, 3253–3260. [Google Scholar] [CrossRef] - Klobes, B.; Staab, T.; Dudzik, E. Early Stages of Decomposition in Al Alloys Investigated by X-Ray Absorption. Phys. Status Solidi (RRL) Rapid Res. Lett.
**2008**, 2, 182–184. [Google Scholar] [CrossRef] - Klobes, B.; Korff, B.; Balarisi, O.; Eich, P.; Haaks, M.; Kohlbach, I.; Maier, K.; Sotong, R.; Staab, T. Defect Investigations of Micron Sized Precipitations in Al Alloys. J. Phys. Conf. Ser.
**2011**, 262, 012030. [Google Scholar] [CrossRef] - Wang, S.; Starink, M. Precipitations and Intermetallic Phases in Precipitation Hardening Al-Cu-Mg-(Li) Based Alloys. Int. Mater. Rev.
**2005**, 50, 193–215. [Google Scholar] [CrossRef] - Staab, T.; Zamponi, C.; Haaks, M.; Modrow, H.; Maier, K. Atomic Structure of pre-Guinier-Preston Zones in Al-Alloys. Phys. Status Solidi (RRL) Rapid Res. Lett.
**2007**, 1, 172–174. [Google Scholar] [CrossRef] - Makkonen, I.; Hakala, M.; Puska, M. Calculation of Valence Electron Momentum Densities using the Projector Augmented-Wave Method. J. Phys. Chem. Solids
**2005**, 66, 1128–1135. [Google Scholar] [CrossRef] - Rehr, J.; Albers, R. Theoretical Approaches to X-Ray Absorption Fine Structure. Rev. Mod. Phys.
**2000**, 72, 621–654. [Google Scholar] [CrossRef] - Kresse, G.; Furthmüller, J. Efficiency of ab initio Total Energy Calculations for Metals and Semiconductors using a Plane-Wave Basis Set. Comput. Mater. Sci.
**1993**, 6, 15–50. [Google Scholar] [CrossRef] - Kresse, G.; Furthmüller, J. Efficient Iterative Schemes for ab initio Total-Energy Calculations using a Plane-Wave Basis Set. Phys. Rev.
**1996**, B54, 11169–11186. [Google Scholar] [CrossRef] - Monkhorst, H.; Pack, J. Special Points for Brillouin-Zone Integrations. Phys. Rev.
**1976**, B13, 5188–5192. [Google Scholar] [CrossRef] - Soler, J.; Artacho, E.; Gale, J.; García, A.; Junquera, J.; Ordejón, P.; Sánchez-Portal, D. The SIESTA Method for ab initio Order-N Materials Simulation. J. Phys. Condens. Matter
**2002**, 14, 2745–2779. [Google Scholar] [CrossRef] - Kohlbach, I.; Korff, B.; Staab, T. (Meta-) Stable Phases and Pre-Guinier-Preston Zones in AlCu-Alloys Constructed from ab initio Relaxed Atomic Positions—Comparison to Experimental Methods. Phys. Status Solidi B
**2010**, 247, 2168–2178. [Google Scholar] [CrossRef] - Wolfertz, I. Ab initio Untersuchungen an frühen Ausscheidungsphasen der Aluminium(-Magnesium-) Kupfer-Legierungen. Ph.D. Thesis, HISKP, University Bonn, Bonn, Germany, 2014. [Google Scholar]
- Mantl, S.; Triftshäuser, W. Defect Annealing Studies on Metals by Positron Annihilation and Electrical Resistivity Measurements. Phys. Rev.
**1978**, B17, 1645–1652. [Google Scholar] [CrossRef] - Staab, T.; Krause-Rehberg, R.; Vetter, B.; Kieback, B. The influence of Microstructure on the Sintering Process in Crystalline Metal Powders investigated by Positron Lifetime Spectroscopy: Part I: Electrolytic and Spherical Copper Powder. J. Phys. Condens. Matter
**1999**, 11, 1757–1786. [Google Scholar] [CrossRef] - Rajainmäki, H.; Linderoth, S. Stage II Recovery in Proton-Irradiated Aluminum Studied by Positrons. J. Phys. Condens. Matter
**1990**, 2, 6623–6630. [Google Scholar] [CrossRef] - Konno, T.; Kawasaki, M.; Hiragi, K. Characterization of Guinier-Preston Zones by High-Angle Annular Detector Dark-Field Scanning Transmission Electron Microscopy. JEOL News
**2001**, 36E, 14–17. [Google Scholar] - Hardy, H. Report on Precipitation. Prog. Met. Phys.
**1954**, 5, 143–278. [Google Scholar] [CrossRef] - Baur, R.; Gerold, V. Entmischungsvorgänge im System Aluminium-Kupfer. Zeitschrift für Metallkunde
**1966**, 57, 181–186. [Google Scholar] - Gerold, V.; Schweizer, W. Die Kinetik von Entmischungsvorgängen in übersättigten Aluminium- Zink-Mischkristallen. Zeitschrift für Metallkunde
**1961**, 52, 76–86. [Google Scholar] - Gerold, V. Die Zonenbildung in Aluminium-Zink-Legierungen. Phys. Status Solidi A
**1961**, 1, 37–49. [Google Scholar] [CrossRef] - Dlubek, G.; Kabisch, O.; Brümmer, O.; Löffler, H. Precipitation and Dissolution Processes in Age-Hardenable Al Alloys—A Comparison of Positron Annihilation and X-Ray Small Angle Scattering Investigations—I. Al-Zn(x) (x = 3, 4.5, 6, 10, 18 at.%). Phys. Status Solidi A
**1979**, 55, 509–518. [Google Scholar] [CrossRef] - Krause, R.; Dlubek, G.; Wendrock, G. Structural Changes during Post-Ageing of an Al-Zn (15 at.%) Alloy at 100 °C Studied by Positron Annihilation, Small Angle X-Ray Scattering and Microhardness Measurements. Cryst. Res. Technol.
**1985**, 20, 1495–1501. [Google Scholar] [CrossRef] - Gläser, U.; Dlubek, G.; Krause, R. Vacancies and Precipitates in Al—1.9at % Cu Studied by Positrons. Phys. Status Solidi A
**1991**, 163, 337–343. [Google Scholar] [CrossRef] - Fontaine, A.; Lagarde, P.; Naudon, A.; Raoux, D.; Spanjaard, D. EXAFS Studies on Al-Cu Alloys. Philos. Mag. B
**1979**, 40, 17–30. [Google Scholar] [CrossRef] - Staab, T.; Haugk, M.; Frauenheim, T.; Leipner, H. Magic Number Vacancy Clusters in GaAs—Structure and Positron Lifetime Studies. Phys. Rev. Lett.
**1999**, 83, 5519–5522. [Google Scholar] [CrossRef]

**Figure 1.**Configuration of Cu-atoms in 2D platelets on the $\left\{100\right\}$-plane in fcc Al. The Cu and Al atoms are shown by red and grey spheres, respectively. The numbering indicates how the Cu-platelets were assumed to grow. The left and right patterns show the sequences 1 and 2 used in the calculations, respectively.

**Figure 2.**Energy gain during Cu-cluster growth for a supercell of 108 atoms in sequences 1 and 2. (

**left**) The energy gain due to the last attached Cu atom, (

**right**) the total energy gain per Cu atom in the growing cluster. Sequences 1 and 2 are explained in Figure 1.

**Figure 3.**Energy gain during Cu-cluster growth. Results corresponding to supercells of 108, 128, and 192 atoms are compared. (

**left**) Energy gain due to the last Cu atom attached, and (

**right**) total energy gain per Cu-atom of a growing cluster. Sequence 1 is explained in Figure 1.

**Figure 4.**Energy gain during Cu-cluster growth. The results corresponding to the supercells of 108, 128, and 192 atoms are compared. (

**left**) Energy gain of the last Cu atom attached, (

**right**) total energy gain per Cu-atom of a growing cluster. Sequence 2 is explained in Figure 1.

**Figure 5.**Relaxation patterns of growing clusters. (

**left**) Two copper atoms (red spheres) on 1NN position, (

**right**) five Cu-atoms arranged as a platelet on the $\left\{100\right\}$-plane. The Al atoms having two or more bonds to Cu-atoms are plotted in dark-grey color. The relaxation of the Al-layer above and below towards the Cu-atoms on the $\left\{100\right\}$-plane clearly increases with the number of agglomerated Cu-aotms.

**Figure 6.**Total energies calculated by using static (atoms fixed) and relaxed configurations of a supercell of 108 atoms.

**Figure 7.**Binding energies of Zn atoms in 2D and 3D Zn clusters. (

**left**) The binding energy for the last attached Zn atom. (

**right**) The binding energy per Zn atom in the cluster.

**Table 1.**Comparison with experimental results: Formation energies for mono- ${H}_{\mathrm{V}}^{\mathrm{F}}$ and di-vacancies ${H}_{2\mathrm{V},\mathrm{X}}^{\mathrm{F}}$ in the nearest neighbor (X = 1NN) and next nearest neighbor (X = 2NN) positions in fcc Al. The binding energies ${H}_{2\mathrm{V},\mathrm{X}}^{\mathrm{b}}$ of the two vacancies in the two configurations are also given. Positive and negative binding energies indicate repulsion and binding, respectively. (SIESTA results: see [34]).

Method | Volume Relax | MP-Mesh | Atoms | ${\mathit{H}}_{\mathbf{V}}^{\mathbf{F}}$ | ${\mathit{H}}_{2\mathbf{V},1\mathbf{NN}}^{\mathbf{F}}$ | ${\mathit{H}}_{2\mathbf{V},2\mathbf{NN}}^{\mathbf{F}}$ | ${\mathit{H}}_{2\mathbf{V},1\mathbf{NN}}^{\mathbf{b}}$ | ${\mathit{H}}_{2\mathbf{V},2\mathbf{NN}}^{\mathbf{b}}$ |
---|---|---|---|---|---|---|---|---|

(eV) | (eV) | (eV) | (eV) | (eV) | ||||

VASP-LDA | yes | $6\times 6\times 6$ | 64 | 0.71 | — | — | — | — |

VASP-LDA | no | $6\times 6\times 6$ | 64 | 0.713 | 1.506 | 1.409 | +0.081 | −0.016 |

VASP-LDA | no | $6\times 6\times 6$ | 108 | 0.714 | 1.489 | 1.421 | +0.061 | −0.007 |

VASP-GGA | no | $6\times 6\times 6$ | 108 | 0.66 | — | — | — | — |

SIESTA-DZP | no | $3\times 3\times 3$ | 108 | 0.64 | — | — | — | — |

Exp. [16] | — | — | — | 0.67 |

**Table 2.**Solubility enthalpy $\Delta {H}_{\mathrm{mix}}$ of Cu in Al calculated by using Equation (2) and different supercell sizes.

Supercell Size (atom) | $\mathbf{\Delta}{\mathit{H}}_{\mathbf{mix}}$ (meV) |
---|---|

108 | −50.5 |

128 | −54.2 |

144 | $-53.0$ |

**Table 3.**Binding energy of two Cu solute atoms in Al on nearest neigbor positions in fcc Al. The c-direction is perpendicular to the habit plane of the Cu atoms. Negative signs indicate binding.

Scheme | Number Atoms | Size Unit Cells | k-points | ${\mathit{E}}_{\mathbf{bind}}$ (meV) |
---|---|---|---|---|

LDA | 108 | $3\times 3\times 3$ | $4\times 4\times 4$ | −50.3 |

LDA | 128 | $4\times 4\times 2$ | $4\times 4\times 8$ | −46.3 |

LDA | 144 | $3\times 3\times 4$ | $4\times 4\times 4$ | −56.2 |

LDA | 192 | $4\times 4\times 3$ | $3\times 3\times 6$ | −54.7 |

GGA | 108 | $3\times 3\times 3$ | $6\times 6\times 6$ | −51.5 |

**Table 4.**Binding energies for agglomerates of Cu atoms in 1D, 2D, and 3D configurations. The calculation employed the 108 atom supercell. Given is the total binding energy, the binding energy per Cu-atom, and the binding energy of the ‘last’ Cu atom specified in Figure 1. We give here the energy with an accuracy of $0.1\phantom{\rule{0.166667em}{0ex}}\mathrm{meV}$, which is only of internal numerical relevance. The numbering is according to Figure 1 left.

Agglomerate | atom no. | Spatial | ${\mathit{E}}_{\mathbf{bind}}$ (meV) | ${\mathit{E}}_{\mathbf{bind}}$ (meV) | ${\mathit{E}}_{\mathbf{bind}}$ (meV) |
---|---|---|---|---|---|

structure | extension | cluster | per Cu | last Cu | |

(a) 2 Cu 1NN on $\left(100\right)$-plane | 1, 2 | 2D | −50.3 | −25.1 | −50.2 |

(b) 2 Cu 2NN on $\left(100\right)$-plane | 1, 4 | 2D | −9.6 | −4.8 | −9.6 |

(c) 3 Cu in-line on $\left(100\right)$-plane | 6, 7, 8 | 1D | −95.2 | −31.7 | −45.0 |

(d) 3 Cu triangle on $\left(100\right)$-plane | 1, 2, 3 | 2D | −134.7 | −44.9 | −84.4 |

(e) 3 Cu triangle on $\left(111\right)$-plane | – | 2D | − 97.4 | −32.5 | −47.1 |

(f) 4 Cu rectangle on $\left(100\right)$-plane | 1, 2, 3, 4 | 2D | −344.7 | −86.2 | −210.0 |

(g) 4 Cu triangle on $\left(100\right)$-plane | 1, 2, 3, 5 | 2D | −206.1 | −51.5 | −71.4 |

(h) 4 Cu tetrahedron in space | – | 3D | +53.0 | +13.2 | +150.4 |

Type | Size (atoms) | Size (Unit Cell) | MP-mesh |
---|---|---|---|

standard | 108 | $3\times 3\times 3$ | $4\times 4\times 4$ |

flattened | 128 | $4\times 4\times 2$ | $4\times 4\times 6$ |

elevated | 144 | $3\times 3\times 4$ | $3\times 3\times 2$ |

widened | 192 | $4\times 4\times 3$ | $2\times 2\times 3$ |

© 2018 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Staab, T.E.M.; Folegati, P.; Wolfertz, I.; Puska, M.J.
Stability of Cu-Precipitates in Al-Cu Alloys. *Appl. Sci.* **2018**, *8*, 1003.
https://doi.org/10.3390/app8061003

**AMA Style**

Staab TEM, Folegati P, Wolfertz I, Puska MJ.
Stability of Cu-Precipitates in Al-Cu Alloys. *Applied Sciences*. 2018; 8(6):1003.
https://doi.org/10.3390/app8061003

**Chicago/Turabian Style**

Staab, Torsten E. M., Paola Folegati, Iris Wolfertz, and Martti J. Puska.
2018. "Stability of Cu-Precipitates in Al-Cu Alloys" *Applied Sciences* 8, no. 6: 1003.
https://doi.org/10.3390/app8061003